1 A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S Volume Issue 2 DOI: /v G. WNUK EXPERIMENTAL STUDY ON THERMODYNAMICS OF THE Cu-Ni-Sn- LIQUID ALLOYS BADANIA TERMODYNAMICZNE CIEKŁYCH STOPÓW Cu-Ni-Sn- The activity of in dilute Cu-Ni-Sn- alloys has been determined by the method of equilibrium saturation with metal vapour at T= 1398, 1448 and 1473 K. As the method of equilibrium saturation is a comparative one, it is necessary to have an appropriate reference mixture. The Cu- alloy was accepted as the reference mixture. The interaction parameters ε, εni and ε Sn were determined by the least squares method. Keywords: activity, interaction parameter, multicomponent alloys Aktywność bizmutu w ciekłych rozcieńczonych stopach Cu-Ni-Sn- w temperaturze T=1398, 1448 i 1473K wyznaczono porównawczą metodą równowagowego nasycania, stosując stop Cu- jako roztwór wzorcowy. Parametry oddziaływania ε, ε Ni i ε Sn wyznaczono metodą najmniejszych kwadratów. 1. Introduction In recent years much effort was put into developing alternative lead-free solder alloys due to the environmental and health concerns on lead usage. Ternary, quaternary and higher order systems containing Sn, Zn, Sb,, Cu and other elements have been examined, but there remain many systems deserving further investigations. Since many of multicomponent systems where promising Pb-free phases are expected to be found contain and Zn, a thorough examination of systems with these elements should be carried out. This paper presents a part of a general examination of Cu-Ni-X-Y (X, Y = Sn,, Zn, Ti) based alloys in relation to development of lead free solders. There is a lot of experimental data for binary, ternary or quaternary Cu-Ni-X-Y alloys [1-15], but there has been no data for the Cu-Ni-Sn- system and this paper shows the results of experimental work on it. pressure of is much higher than that of other elements, the activity measurements of were carried out by the comparative method of equilibrium vapour saturation, that is a modified isothermal isopiestic method [4,8,10,11]. Apparatus used in experiments is presented in Figure Experiments The analyzed alloys show considerable differences between vapour pressures of their elements. For instance at T=1473K: p Sn = 9.4*10 3 hpa, p Ni = 1.16*10 4 hpa, pcu = 3.95*10 3 hpa, p = hpa . As the vapour Fig. 1. Apparatus for the equilibrium saturation. (1 [Ni-(Ni-Cr)] thermocouple and alundum sheath for thermocouple, 2 graphite blocks, 3 graphite blocks with grooves for alloys, 4 chamber) The Cu-Ni-Sn alloys of different compositions were placed in five grooves of each block and the reference RZESZÓW UNIVERSITY OF TECHNOLOGY, RZESZÓW, 2 W. POLA STR., POLAND
2 306 mixture Cu- was placed in the sixth groove. This alloy was the only source of vapour in the system. Pure cooper was placed in the seventh groove. Three blocks with grooves with alloys were placed between two graphite blocks (Fig.1). That assured constant temperature during heating. The apparatus was placed in a tube made of extra-fine, creep resistant steel, which served as a chamber. The air from the chamber was pumped out and argon was let in. The argon pressure (20 hpa for 1398K, 40hPa for 1448K and 50 hpa for 1473K) guaranteed free migration of vapour between alloys. The chamber with grooves with alloys was placed inside an isothermal zone of the resistant furnace and kept at a fixed temperature (1398, 1448 and 1473K) and alloys saturated with the bismuth vapour for a time necessary to attain equilibrium between (g) in all alloys (2h). At the equilibrium state, the activity of was the same in all alloys inside a closed system: a (Cu ) = a (Cu Ni Sn ) (1) Equal concentration in both Cu- alloys (grooves sixth and seventh) guaranteed equilibrium attainment. Than, argon was let into a chamber till the pressure reached 900 hpa. As the chamber was taken out from the furnace, bismuth evaporation was stopped and alloys solidified quickly. If the alloys equilibrium compositions and activity coefficient of in the reference Cu- alloy are known, it is possible to calculate the activity coefficient of in the Cu-Ni-Sn- alloy: γ (Cu Ni Sn ) = x (Cu ) γ (Cu ) /x (Cu Ni Sn ) (2) where x (Cu ) and x (Cu Ni Sn ) denote the equilibrium mole fraction of in Cu- and Cu-Ni-Sn- respectively, and γ (Cu ) and γ (Cu Ni Sn ) are the corresponding activity coefficients of. Samples of the reference and the studied alloys of 3.5 g were prepared by melting carefully weighed masses of metals at an argon pressure of 0.1 Pa. The equilibrium compositions of the alloys were determined by the weighing. The accuracy of weighing was ±10 4 g. The quantities determined experimentally, i.e. the argon pressure and the equilibration time were meant to ensure the attainment of equilibrium between (g) in the reference and the studied mixture. It was established that for the temperature 1398, 1448 and 1473 K the time necessary to reach equilibrium was 2 hours and the argon pressure was 20, 40 or 50 hpa. 3. Results The activity of bismuth in Cu-Ni-Sn- at 1398, 1448 and 1473 K was determined by the equilibrium saturation method. The activity coefficient of bismuth (γ Bι )p in this alloy was calculated from the equation (2). The experimental values of activity coefficient are presented in Tables 1-3. TABLE 1 Experimental values of bismuth activity coefficient γ at 1398K Lp Cu-Ni-Sn- Cu- x Ni x Sn x γ x γ
3 307 TABLE 2 Experimental values of bismuth activity coefficient γ at 1448K TABLE 3 Experimental values of bismuth activity coefficient γ at 1473K Lp Cu-Ni-Sn- Cu- Lp Cu-Ni-Sn- Cu- x Ni x Sn x γ x γ x Ni x Sn x γ x γ
4 308 For describing the activity coefficient of bismuth (γ ) in the reference mixture (Cu-) the equation proposed by Teppo  with the following Redlich-Kister  parameters was used: 0 L L,Cu = T [J/mol] 1 L L,Cu = T [J/mol] (3) As the solutions are dilute ones, they can be described by means of the Wagner equation : lnγ = lnγ 0 +ε x +ε Sn x Sn+ε Ni x Ni (4) where γ w is the activity coefficient of in Cu-Ni-Sn- at x 0, ε = ( lnγ / x ), x 0, x Ni 0, x Sn 0 is the interaction parameter of in Cu-Ni-Sn-, ε Sn=( lnγ / x Sn ) x 0, x Sn 0, x Ni 0 is the interaction parameter of Sn in Cu-Ni-Sn- and ε Ni= ( lnγ / x Ni ), x 0, x Ni 0, x Sn 0 is the interaction parameter of Ni in Cu-Ni-Sn-. In the equation (4) values of mole fractions of components and bismuth activity coefficient were determined experimentally, whereas values of lnγ 0, ε, εni, εsn were calculated by means of the least-squares method. On the basis of the experimental results, the following expressions for the activity coefficients were obtained: T = 1398K: Fig. 2. Experimental and calculated values of γ for x Ni = T = 1448K: lnγ = x x Sn 1.58x Ni (5) T = 1473 K: lnγ = x x Sn 1.55x Ni (6) Fig. 3. Experimental and calculated values of γ for x Ni = lnγ = x x Sn 1.25x Ni (7) Values of interaction parameters are presented in Table 4. Values of interaction parameters TABLE 4 T [K] ln γ 0 ε ε Sn ε Ni The comparision between the calculated and experimental activity coefficients for some fixed Ni concentrations at 1398K is presented in Figs Fig. 4. Experimental and calculated values of γ for x Ni =0.0278
5 309 When there is accepted x Ni =0 in Eq. (6), the results obtained are in good agreement with results for the ternary Cu-Sn- alloys obtained on the basis of Eq.(12) , see Fig. 7. lnγ = x x Sn (12) Fig. 5. Experimental and calculated values of γ for x Ni = The temperature dependence of interaction parameters is presented in equations (8-11) and Figure 6. lnγ 0 = T (8) ε = T (9) ε Sn = T (10) ε Ni = T (11) Fig. 7. Calculated bismuth activity coefficient γ in Cu-Sn- and Cu-Ni-Sn- for x Ni =0 4. Conclusions Using the vapour saturation method, the activities in Cu-Ni-Sn- alloys at the temperature 1398, 1448 and 1473K were measured and interaction parameters were calculated. Theses results, combined with other measurements carried on within the frame of the COST action MP0602 Advanced Solder Materials for High Temperature Application HISOLD, a group project Design, Process and Control in a Multiscale domain of Cu-Ni-X-Y (X, Y = Sn,, Zn) Based Alloys allow to construct thermodynamic database that may be useful for the computer modelling of the system and to determine compositions suitable for practical applications as soldering materials. Fig. 6. The influence of temperature on the interaction parameters We can see from Table 4, Fig. 6 and the equations (8-11) that the values of interaction parameters do not change significantly with the temperature. As the value of ε Ni is close to 1 (1.58, 1.55, 1.25), the nickel influence on activity is smaller than the influence of other components (ε <-5 and ε Sn >4). Acknowledgements The work was supported by the Polish Ministry of Science and Higher Education (Project no. N N ). It was conducted within the frame of the European action COST MP0602 Advanced Solder Materials for High Temperature Application (HISOLD), project Design, Process and Control in a Multiscale Domain of Cu-Ni-X-Y (X,Y = Sn,, Zn, Ti) Based Alloys.
6 310 REFERENCES  C. C h o u, S. C h e n, Acta Materialia 54, (2006).  J. M i e t t i n e n, Metall. Mater. Trans. 33A, (2002).  G. G h o s h, Metall. Trans. 30A, (1999).  G.P. V a s s i l e v, J. R o m a n o w s k a, G. W n u k, Int. J. Mat. Res. 98(6), 1-6 (2007).  O. T e p p o, J. N i e m w e l a, P. T a s k i n e n, Thermochimica Acta 1973, (1990).  J. V i z d a l, M.H. B r a g a, A. K r o u p a, K.W. R i c h t e r, D. S o a r e s, L.F. M a l h e i r o s, J. F e r - r i e r a, CALPHAD 31, (2007).  J. M i e t t i n e n, CALPHAD 27, (2003).  G. W n u k, J. R o m a n o w s k a, Arch. Metall. Mater. 51(4), (2006).  M.H. B r a g g a, J. V i z d a l, A. K r o u p a, J. F e r - r i e r a, D. S o a r e s, L.K. M a l h e i r o s, CALPHAD 31, (2007).  J. R o m a n o w s k a, G. W n u k, P. R o m a n o w s - k i, Arch. Met. Mater. 53(3), (2008).  G. W n u k, J. R o m a n o w s k a, Arch. Met. Mater. 29(4), (2004).  H. L i u, J. W a n g, Z.P. J i n, CALPHAD 28, (2004).  G.P. V a s s i l e v, K. I s h i d a, J. Alloys Compounds 376, (2004).  G.P. V a s s i l e v, K.I. L i l o v a, J.C. G a c h o n, J.Alloys Compounds 469, (2009).  Y. H u a n g, S. C h e n, C. C h o u, W. G i e r l o t k a, J. Alloys Compounds 477, (2009).  O. K u b a s c h e w s k i, Alcock C.: Metallurgical Thermochemistry, Pergamon Press, Oxford,  O. R e d l i c h, T. K i s t e r, Ind. Enging. Chem. 40, (1948).  K. W a g n e r, Thermodynamics of alloys Addison-Wesley Reading, Mass Received: 10 December 2010.